General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.77 g/cm³ Show Material materials with Density of 7.77 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 211.67 - 218 GPa Show Material materials with Elastic modulus of 211.67 - 218 GPa |

95.0 °C | 208.22 GPa Show Material materials with Elastic modulus of 208.22 GPa | |

100.0 °C | 213 - 214 GPa Show Material materials with Elastic modulus of 213 - 214 GPa | |

150.0 °C | 204.77 GPa Show Material materials with Elastic modulus of 204.77 GPa | |

200.0 °C | 206 - 207 GPa Show Material materials with Elastic modulus of 206 - 207 GPa | |

205.0 °C | 200.64 GPa Show Material materials with Elastic modulus of 200.64 GPa | |

260.0 °C | 196.5 GPa Show Material materials with Elastic modulus of 196.5 GPa | |

300.0 °C | 198 - 199 GPa Show Material materials with Elastic modulus of 198 - 199 GPa | |

315.0 °C | 191.67 GPa Show Material materials with Elastic modulus of 191.67 GPa | |

370.0 °C | 186.85 GPa Show Material materials with Elastic modulus of 186.85 GPa | |

400.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | |

425.0 °C | 181.33 GPa Show Material materials with Elastic modulus of 181.33 GPa | |

485.0 °C | 175.82 GPa Show Material materials with Elastic modulus of 175.82 GPa | |

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | |

540.0 °C | 170.3 GPa Show Material materials with Elastic modulus of 170.3 GPa | |

595.0 °C | 165.47 GPa Show Material materials with Elastic modulus of 165.47 GPa | |

600.0 °C | 167 - 168 GPa Show Material materials with Elastic modulus of 167 - 168 GPa | |

650.0 °C | 159.96 GPa Show Material materials with Elastic modulus of 159.96 GPa | |

700.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

760.0 °C | 137.21 GPa Show Material materials with Elastic modulus of 137.21 GPa | |

Elongation | 20.0 °C | 20 % Show Material materials with Elongation of 20 % |

Elongation, transverse | 20.0 °C | 18 % Show Material materials with Elongation, transverse of 18 % |

Poisson's ratio | 20.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] |

95.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

150.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

205.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

260.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

315.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

370.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

425.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

485.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

540.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

595.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

650.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

760.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 81.7 GPa Show Material materials with Shear modulus of 81.7 GPa |

95.0 °C | 80.32 GPa Show Material materials with Shear modulus of 80.32 GPa | |

150.0 °C | 78.95 GPa Show Material materials with Shear modulus of 78.95 GPa | |

205.0 °C | 77.22 GPa Show Material materials with Shear modulus of 77.22 GPa | |

260.0 °C | 75.5 GPa Show Material materials with Shear modulus of 75.5 GPa | |

315.0 °C | 73.77 GPa Show Material materials with Shear modulus of 73.77 GPa | |

370.0 °C | 71.71 GPa Show Material materials with Shear modulus of 71.71 GPa | |

425.0 °C | 69.64 GPa Show Material materials with Shear modulus of 69.64 GPa | |

485.0 °C | 67.22 GPa Show Material materials with Shear modulus of 67.22 GPa | |

540.0 °C | 65.16 GPa Show Material materials with Shear modulus of 65.16 GPa | |

595.0 °C | 63.43 GPa Show Material materials with Shear modulus of 63.43 GPa | |

650.0 °C | 60.33 GPa Show Material materials with Shear modulus of 60.33 GPa | |

760.0 °C | 51.71 GPa Show Material materials with Shear modulus of 51.71 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 590 - 740 MPa Show Material materials with Tensile strength of 590 - 740 MPa |

100.0 °C | 550 MPa Show Material materials with Tensile strength of 550 MPa | |

150.0 °C | 525 MPa Show Material materials with Tensile strength of 525 MPa | |

200.0 °C | 500 MPa Show Material materials with Tensile strength of 500 MPa | |

250.0 °C | 490 MPa Show Material materials with Tensile strength of 490 MPa | |

300.0 °C | 480 MPa Show Material materials with Tensile strength of 480 MPa | |

350.0 °C | 460 MPa Show Material materials with Tensile strength of 460 MPa | |

400.0 °C | 430 MPa Show Material materials with Tensile strength of 430 MPa | |

450.0 °C | 405 MPa Show Material materials with Tensile strength of 405 MPa | |

500.0 °C | 360 MPa Show Material materials with Tensile strength of 360 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 590 - 740 MPa Show Material materials with Tensile strength, transverse of 590 - 740 MPa |

Yield strength Rp0.2 | 20.0 °C | 390 MPa Show Material materials with Yield strength Rp0.2 of 390 MPa |

100.0 °C | 375 MPa Show Material materials with Yield strength Rp0.2 of 375 MPa | |

150.0 °C | 365 MPa Show Material materials with Yield strength Rp0.2 of 365 MPa | |

200.0 °C | 355 MPa Show Material materials with Yield strength Rp0.2 of 355 MPa | |

250.0 °C | 345 MPa Show Material materials with Yield strength Rp0.2 of 345 MPa | |

300.0 °C | 335 MPa Show Material materials with Yield strength Rp0.2 of 335 MPa | |

350.0 °C | 325 MPa Show Material materials with Yield strength Rp0.2 of 325 MPa | |

400.0 °C | 315 MPa Show Material materials with Yield strength Rp0.2 of 315 MPa | |

450.0 °C | 295 MPa Show Material materials with Yield strength Rp0.2 of 295 MPa | |

500.0 °C | 275 MPa Show Material materials with Yield strength Rp0.2 of 275 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 390 MPa Show Material materials with Yield strength Rp0.2, transverse of 390 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1E-5 1/K Show Material materials with Coefficient of thermal expansion of 1E-5 1/K | |

20.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | ||

100.0 °C | 1.12E-5 - 1.13E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.12E-5 - 1.13E-5 1/K | ||

200.0 °C | 1.16E-5 - 1.18E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.16E-5 - 1.18E-5 1/K | ||

300.0 °C | 1.2E-5 - 1.23E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.2E-5 - 1.23E-5 1/K | ||

400.0 °C | 1.23E-5 - 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.23E-5 - 1.27E-5 1/K | ||

425.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

485.0 °C | 1.22E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.22E-5 1/K | ||

500.0 °C | 1.26E-5 - 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.26E-5 - 1.3E-5 1/K | ||

540.0 °C | 1.23E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.23E-5 1/K | ||

595.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

600.0 °C | 1.29E-5 - 1.32E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 - 1.32E-5 1/K | ||

650.0 °C | 1.27E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.27E-5 1/K | ||

700.0 °C | 1.33E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.33E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1382 - 1529 °C Show Material materials with Melting point of 1382 - 1529 °C | Typical for Chromium Molybdenum Steel | |

Specific heat capacity | 20.0 °C | 429 J/(kg·K) Show Material materials with Specific heat capacity of 429 J/(kg·K) | |

100.0 °C | 464 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 464 - 500 J/(kg·K) | ||

200.0 °C | 492 - 530 J/(kg·K) Show Material materials with Specific heat capacity of 492 - 530 J/(kg·K) | ||

300.0 °C | 511 - 560 J/(kg·K) Show Material materials with Specific heat capacity of 511 - 560 J/(kg·K) | ||

400.0 °C | 531 - 610 J/(kg·K) Show Material materials with Specific heat capacity of 531 - 610 J/(kg·K) | ||

500.0 °C | 554 - 680 J/(kg·K) Show Material materials with Specific heat capacity of 554 - 680 J/(kg·K) | ||

600.0 °C | 585 - 780 J/(kg·K) Show Material materials with Specific heat capacity of 585 - 780 J/(kg·K) | ||

700.0 °C | 626 J/(kg·K) Show Material materials with Specific heat capacity of 626 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 20.7 W/(m·K) Show Material materials with Thermal conductivity of 20.7 W/(m·K) | |

100.0 °C | 22.6 - 23 W/(m·K) Show Material materials with Thermal conductivity of 22.6 - 23 W/(m·K) | ||

200.0 °C | 24 - 24.4 W/(m·K) Show Material materials with Thermal conductivity of 24 - 24.4 W/(m·K) | ||

300.0 °C | 25.8 - 26 W/(m·K) Show Material materials with Thermal conductivity of 25.8 - 26 W/(m·K) | ||

400.0 °C | 26.9 - 27 W/(m·K) Show Material materials with Thermal conductivity of 26.9 - 27 W/(m·K) | ||

500.0 °C | 27.8 - 28 W/(m·K) Show Material materials with Thermal conductivity of 27.8 - 28 W/(m·K) | ||

600.0 °C | 28.5 - 29 W/(m·K) Show Material materials with Thermal conductivity of 28.5 - 29 W/(m·K) | ||

700.0 °C | 28.8 W/(m·K) Show Material materials with Thermal conductivity of 28.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 6.2 mm²/s Show Material materials with Thermal diffusivity of 6.2 mm²/s | |

100.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

200.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

300.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

400.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

500.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 5.03E-7 Ω·m Show Material materials with Electrical resistivity of 5.03E-7 Ω·m |

100.0 °C | 5.67E-7 - 5.7E-7 Ω·m Show Material materials with Electrical resistivity of 5.67E-7 - 5.7E-7 Ω·m | |

200.0 °C | 6.47E-7 - 6.5E-7 Ω·m Show Material materials with Electrical resistivity of 6.47E-7 - 6.5E-7 Ω·m | |

300.0 °C | 7.27E-7 - 7.3E-7 Ω·m Show Material materials with Electrical resistivity of 7.27E-7 - 7.3E-7 Ω·m | |

400.0 °C | 8.09E-7 - 8.1E-7 Ω·m Show Material materials with Electrical resistivity of 8.09E-7 - 8.1E-7 Ω·m | |

500.0 °C | 8.9E-7 Ω·m Show Material materials with Electrical resistivity of 8.9E-7 Ω·m | |

600.0 °C | 9.7E-7 - 9.72E-7 Ω·m Show Material materials with Electrical resistivity of 9.7E-7 - 9.72E-7 Ω·m | |

700.0 °C | 1.06E-6 Ω·m Show Material materials with Electrical resistivity of 1.06E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.15 % Show Material materials with Carbon of 0.15 % |

Chromium | 8 - 10 % Show Material materials with Chromium of 8 - 10 % |

Manganese | 0.3 - 0.6 % Show Material materials with Manganese of 0.3 - 0.6 % |

Molybdenum | 0.9 - 1.1 % Show Material materials with Molybdenum of 0.9 - 1.1 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.25 - 1 % Show Material materials with Silicon of 0.25 - 1 % |

Sulfur | 0.03 % Show Material materials with Sulfur of 0.03 % |

Do you have a technical question or need more information about this material?

Post it as a comment below and receive answers from engineers and other community members.